Lecture #14. ANNOUNCEMENTS Reader with reference material from Howe & Sodini and from Rabaey et al available at Copy Central on Hearst Ave. near Euclid OUTLINE Semiconductor materials Properties of silicon Doping Reading Howe & Sodini: Ch. 2.1-2.4.1. V. I. _. +. W. t.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Howe & Sodini: Ch. 2.1-2.4.1
where r is the resistivityElectrical Resistance
High resistivity => “insulator”
Intermediate resistivity => “semiconductor”
Generally, the semiconductor material used in integrated-circuit devices is crystalline
In recent years, however, non-crystalline semiconductors have become commercially very importantWhat is a Semiconductor?
polycrystalline amorphous crystalline
1s, 2s, 2p orbitals filled by 10 electrons
3s, 3p orbitals filled by 4 electrons
To minimize the overall energy, the 3s and 3p orbitals hybridize to form 4 tetrahedral 3sp orbitals
Each has one electron and
is capable of forming a bond
with a neighboring atomThe Silicon Atom
= 5.431ÅThe Si Crystal
“diamond cubic” lattice
Silicon is a semiconductor material.
Pure Si has relatively high resistivity at room temperature.
There are 2 types of mobile charge-carriers in Si:
Conduction electronsare negatively charged.
Holesare positively charged. They are an “absence of electrons”.
The concentration of conduction electrons & holes
in a semiconductor can be affected in several ways:
by adding special impurity atoms (dopants)
by applying an electric field
by changing the temperature
by irradiationElectronic Properties of Si
SiConduction Electrons and Holes
When an electron breaks loose and becomes a
conduction electron, a hole is also created.
Note: A hole (along with its associated positive charge) is mobile!
n = number of mobile electrons per cm3
p = number of holes per cm3
ni= intrinsic carrier concentration (#/cm3)
In a pure semiconductor,
n = p = niDefinition of Parameters
an electron falling through 1 V potential = qeV = 1.6 x 10-19 C x
1 V = 1.6 x 10-19 J.
“thermal recombination” semiconductor is heated
“optical recombination” light is emitted
ni 1010 cm-3 at room temperature
Donors: P, As, Sb
Acceptors: B, Al, Ga, InDoping
By substituting a Si atom with a special impurity atom (Column V
or Column III element), a conduction electron or hole is created.
Dopant concentrations typically range from 1014 cm-3 to 1020 cm-3
ND: ionized donor concentration (cm-3)
NA: ionized acceptor concentration (cm-3)
Charge neutrality condition: ND + p = NA + n
At thermal equilibrium, np = ni2 (“Law of Mass Action”)
Note: Carrier concentrations depend on net dopant concentration (ND - NA) !
andN-type and P-type Material
If ND >> NA(so that ND – NA >> ni):
n >> p material is “n-type”
If NA >> ND(so that NA – ND >> ni):
p >> n material is “p-type”
intrinsic semiconductor: “undoped” semiconductor
electrical properties are native to the material
extrinsic semiconductor: doped semiconductor
electrical properties are controlled by the added impurity atoms
donor: impurity atom that increases the electron concentration
group V elements (P, As)
acceptor: impurity atom that increases the hole concentration
group III elements (B, In)
n-type material: semiconductor containing more electrons than holes
p-type material: semiconductor containing more holes than electrons
majority carrier: the most abundant carrier in a semiconductor sample
minority carrier: the least abundant carrier in a semiconductor sample
~107 cm/s @ 300K
pDrift Velocity and Carrier Mobility
Mobile charge-carrier drift velocity is proportional to applied E-field:
| v | = mE
m is the mobility
Note: Carrier mobility depends on total dopant concentration (ND + NA) !
The current density J is the current per unit area
(J = I/ A ; A is the cross-sectional area of the conductor)
If we have N positive charges per unit volume moving with average speed v in the +x direction, then the current density in the +x direction is just J = qNv
2 x1016 holes/cm3 moving to the right at 2 x104 cm/sec
J = 1.6x10-19 x2x1016 x 2x104 = 64 A/cm2
Suppose this occurs in a conductor 2 mm wide and 1 mm thick:
I = J x A = 64 x (2x10-4 x1x10-4)
= 1.28 mA
hole current density:Electrical Conductivity s
When an electric field is applied, current flows due to drift of mobile electrons and holes:
total current density:
for p-type mat’lElectrical Resistivity r
From mvs. ( NA + ND ) plotExample
Consider a Si sample doped with 1016/cm3 Boron.
What is its resistivity?
NA = 1016/cm3 , ND= 0 (NA >> ND p-type)
p 1016/cm3 and n 104/cm3
Consider the same Si sample, doped additionally
with 1017/cm3 Arsenic. What is its resistivity?
NA = 1016/cm3, ND= 1017/cm3 (ND>>NA n-type)
n 9x1016/cm3 and p 1.1x103/cm3
The sample is converted to n-type material by adding more donors than acceptors, and is said to be “compensated”.
Rs is the resistance when W = L
(L, W, t = length, width, thickness)
R = Rs
R = Rs/2
R = 2Rs
R = 3Rs
The resistivity and thickness t are fixed for each layer in a given manufacturing process
A circuit designer specifies the length L and width W, to achieve a desired resistance R
Example: Suppose we want to design a 5 kW resistor using a layer of material with Rs = 200 W/
Resistor layout (top view)
4 valence electrons per atom
diamond lattice: each atom has 4 nearest neighbors
5 x 1022 atoms/cm3
In a pure Si crystal, conduction electrons and holes are formed in pairs.
Holes can be considered as positively charged mobile particles which exist inside a semiconductor.
Both holes and electrons can conduct current.
Dopants in Si:
Reside on lattice sites (substituting for Si)
Group V elements contribute conduction electrons, and are called donors
Group III elements contribute holes, and are called acceptorsSummary